Microsoft Word  Document5An ecient prediction model of effective
thermal conductivity for metal powder bed in additive manufacturing
Yizhen Zhao
Xi'an Jiaotong University Hang Zhang (
[email protected] )
Xi'an Jiaotong University Jianglong Cai
Xi'an Jiaotong University Shaokun Ji
Xi'an Jiaotong University Dichen Li
Xi'an Jiaotong University
Posted Date: April 7th, 2021
DOI: https://doi.org/10.21203/rs.3.rs287950/v1
License: This work is licensed under a Creative Commons Attribution
4.0 International License. Read Full License
conductivity for metal powder bed in additive manufacturing
Yizhen Zhao, Hang Zhang*, Jianglong Cai, Shaokun Ji, Dichen
Li
State Key Laboratory of Manufacturing Systems Engineering, School
of Mechanical Engineering, Xi’an
Jiaotong University, Xi’an 710049, China
Abstract
The particle accumulation structure is commonly found in diverse
engineering fields, including
additive manufacturing powder, powder metallurgy, advanced reactor,
grain storage and catalyst
bed. The relative thermal conductivity of such structure is an
important parameter to study the heat
transfer behavior of the accumulation. In the study, the key
factors affecting on the thermal
conductivity of the powder is analyzed. Based on the results, the
expression for calculating the
thermal conductivity of the sphere metal powder is successfully
reduced to only one parameter d50
and an efficient calculation model is proposed which can applicate
both in room and high
temperature. Meanwhile, the corresponding error is less than 20.9%
in room temperature and 50%
in high temperature.
Introduction
Thermal conductivity of powder bed has been studied in diverse
industries, including the
energy, chemical, and machinery industries [14]. In the field of
nuclear energy, for example,
modular aircooled high temperature reactors require natural heat
transfer to prevent nucleation and
melting. Studies show that the pebble bed structure can effectively
resolve this problem [5].
Therefore, the thermal conductivity of ball pebble reactors has
become an important design
parameter for nuclear applications. In the machinery industry,
knowing the thermal conductivity of
the powder beds is of significant importance in the design at high
temperature processes (over
200C). Therefore, additional scientific methods are required to
evaluate the effects of the thermal
conductivity of powders and determine the feasibility of powder
beds for high temperature
applications.
The majority of researchers simply use one or a group of equations
to calculate the required
thermal conductivity. Therefore, many researchers have proposed
analytical expressions for
calculating the packing structure of spherical particles [69].
Although many equations are proposed
so far, there is still a great challenge that has not been well
explained yet. In fact, the core factors
affecting the thermal conductivity of particles should be
explained.
The accumulation structure of particles varies significantly with
particle size and distribution.
The stacking structure has a significant influence on the thermal
conductivity [10, 11]. Therefore, if
it is hard to prove that the independent variables in the equation
are strongly correlated with the
thermal conductivity. So, it is a challenge to ensure that the
proposed expression is universal for all
stacking powder structures. According to Majid et al, it is assumed
that by determined the thermal
contact resistance between particles, the particles surface
condition and the average particle size are
the main factors affecting the thermal conductivity [7]. However,
this study shows that this
statement is not accurate.
In this study, the accumulation of particles is classified into two
categories, including equal
particle size accumulation and nonequal particle size
accumulation. This classification is based on
the variance of the particle size distribution. The two situations
present different characteristics.
Considering these two situations, PFC and the selfdeveloped
calculation software are applied to
predict the characteristic parameters of the particle accumulation.
Meanwhile, the core parameters
of the calculation of the thermal conductivity of particles and the
core influencing factors are
determined. According to the results, the equation for predicting
the thermal conductivity of the
metal powder is simplified successfully with only one parameter
(d50). The error is less than 30%,
which shows remarkable improvement of the convenience and accuracy
of the prediction.
Nomenclature
aave Particle average contact area (µm2) Rj Spheresphere interface
thermal
d50 Particle average radius (µm) contact resistance (m2K/W)
ke Effective thermal conductivity(W/mK) RL Heat shrinkage
resistance(m2K/W)
mi Mass inertia of particle(Nm) Rs Peak contact thermal
s
vi Particle velocity (m/s) Rup upper substrate thermal
wi Particle angular velocity (rad/s) resistance(m2K/W)
xi ,x ’ i Original variable and the unified Rx Thermal resistance
of the powder
dimensionless variable region (m2K/W)
Fi Total force applied on particle i (N) T Temperature of powder in
calculation
Ii
Moment inertia of particle (kg m2) ΔQ Energy of heat transfer
(J)
Mi Relevant torques (Nm) Abbreviations
Ra Total thermal resistance(m2K/W) DEM Discrete element model
Rdn Under substrate thermal FDM Finite difference method
resistance (m2K/W) ETCp Effective thermal conductivity
RG Thermal resistance of large of powder
gap (m2K/W) PFC Particle flow code
Rg Thermal resistance of micro TCR Thermal contact resistance
gap (m2K/W) TCs Effective thermal conductivity of
Rgs Interfacial thermal resistance(m2K/W) particle itself
Materials and methods
1.1 Calculation processes of ETCp
The analysis software PFC based on the discrete element method
(DEM) and the computational
analysis software based on the finite difference method (FDM) are
used in the previous study [12,
13]. The simulating process of the thermal conductivity is
described as follows:
Figure1. The whole analysis processes of ETCp
Figure 1 shows that the whole analysis processes are divided into
four steps:
1. Modeling of the particle accumulation process based on the
measured particle distribution or
specially designed particle distribution
2. Extracting particle information and building the discrete model
of the particle accumulation
3. The calculation process based on FDM
4. Analysis of calculation results
Among these steps, the establishment of physical models and the
analysis of results are the key steps.
1.2 Experimental verification method
In this study, the calculation results were verified by comparing
them to the actual thermal
conductivity determined using the hot disk TPS2500S. This
equipment is developed based on
transient plane source (TPS) method, which has a higher temperature
measurement range and
accuracy. Thus, it’s has relatively more applications and research
in recent years [1416].
2. Physical and numerical models
2.1 The particle accumulation model
The calculation of the thermal conductivity of particles should be
performed by the unit cell.
The unit cell is a part of the model extracted from the particle
accumulation model. In the present
study, the PFC software is used to establish the particle
accumulation model. This software is
developed by the discrete element method (DEM). In 1979, Cundall et
al developed the discrete
element method to study the mechanics of granular assemblies [6].
Every degree of freedom of
particles is determined by the explicit solution of Newton's
equations, which is described as the
following:
mivi = ∑ Fi (1) Iiwi = ∑ Mi (2)
in which mi and Ii are the mass and moment of inertia of particle,
and vi and ωi are the particle
velocity and particle angular velocity respectively. ∑Fi represents
the total force applied on particle
i, including body force, contact force between contact particles
and external force applied on the
boundaries of granular assemblies. ∑Mi represents relevant torques
[17].
It should be 1indicated that in the PFC software, the particle size
distribution, the friction
coefficient between particles and mechanical properties of particle
materials can flexibly change to
obtain the corresponding packing structure in the process of the
accumulation modeling. Therefore,
this characteristic provides a great convenience for the subsequent
analysis of the characteristic
parameters of the stacking model.
2.2 The establishment of the particle calculation model
We established a detailed calculation model of the particle heat
transfer (discrete finite
difference model) and calculated the thermal conductivity of the
powder by obtaining the overall
thermal resistance of the model [12].
Figure 2. Thermal resistance composition of the sandwich model.
Figure 2 shows that in the present study, the "upper substrate 
powder  lower substrate"
analysis calculation model is utilized to avoid uneven temperature
distribution at the top and bottom
of the powder. Total powder thermal resistance Rx is composed of
the following five parts: Total
thermal resistance (Ra), upper aluminum plate thermal resistance
(Rup), lower aluminum plate
thermal resistance (Rdn). Therefore:
(3)
Meanwhile, through the heat transfer calculation of the calculation
software, Ra also can be obtained
from the following equation:
(4)
where dt is the time required to reach the stable temperature, s is
heat transfer area, and
is the energy of heat transfer. Therefore, the overall thermal
conductivity of the powder bed
ke is described as the following:
(5)
2.3 Establishment of the heat transfer model
In the present study, the heat transfer calculation model is the
key step to determine Ra. In this
model, as figure3(a) shows the boundary of the model is not
adiabatic, and the heat will transfer
from one side of the boundary to the other through the following
conduction forms: the heat transfer
between particles and the medium gas, the heat transfer between
particles contact and the radiation
heat transfer. Among them, the calculation models of the heat
transfer and radiation heat transfer
between particles and media are mostly classical heat transfer
formulas, which are not discussed in
this study. In this section, the heat transfer between particles is
described.
x a up dn R R R R=  
a up dn [ (  )] /R dt s T T Q= × × D
QD
Q
ì ü í ý î þ
Figure3. The heat transfer forms in particle model and the thermal
resistance composition in particle
contact area.
As the figure 3(b) shows the micro contact area between particles
is composed of the micro
contact on the solid surface and the big gap around. In the powder
bed model, the interfacial thermal
resistance of these micro contact areas hinders the heat transfer
process of the powder bed
significantly. For each independent contact area, the heat transfer
path can be divided into two parts.
One is the heat transfer from the large gap around the micro
contact area and the other is the heat
transfer from the micro contact area. It should be indicated that
the micro contact area is composed
of the internal small gap and the contact of the surface micro peak
[9]. Therefore, it is necessary to
combine the thermal resistance of the large gap with the thermal
resistance of the micro contact area
to characterize the interface thermal resistance of the particle
contact. This simplifies the further
analysis and simulation of the heat transfer process of the whole
powder bed [7]. In summary, the
thermal contact resistance consists of three parts, including Rs,
Rg and RL, which can be determined
as the following:
(6)
Where Rs and RL denote the peak contact thermal resistance in the
microcontact area and the
heat shrinkage resistance between the internal gap and the solid
surface, respectively. Moreover, the
thermal resistance Rs of the micro contact area is mainly affected
by geometry, force acting on it,
and thermal properties. The detailed calculation of each part has
been introduced in the study of
Zhang and will not be discussed in the present study [12].
2.4 Selection of core parameters
Before the parameter analysis, it is necessary to conduct the
primary selection of parameters,
which are as follows:
(1) Temperature T
There is no doubt that the temperature has a great influence on the
thermal conductivity of
particles. Moreover, the thermal conductivity of granular materials
and gap gas itself is greatly
affected by the temperature. Furthermore, the hardness of metals
changes as the temperature
increases. According to the previous study [12], when the
temperature reaches about 0.5Tm, the
accumulation structure of particles change significantly, which
results in the sudden change of the
1 11/ ((1/ R 1/ R ) )
j s g L R R
é ù= + +ë û
(2) Solid fraction ε
The change of densification means that the volume proportion of the
solid changes in a certain
space and the number of contacts between particles changes.
Therefore, it is preliminarily predicted
that the thermal conductivity of the powder is sensitive to the
change of densification [10, 17, 18].
Moreover, the heat transfer between particles mainly depends on the
contact between particles.
Therefore, the influence of the solid fraction on the thermal
conductivity of particles is meaningful.
In the present study, the fric coefficient is adjusted to adjust
the degree of solid fraction.
(3) Particle size d50
The influence of particle size is mainly divided into two aspects.
First, the change of the particle
size induces the variation of solid fraction [3, 19]. Secondly, the
increase of the particle size
increases the average contact area of particles. Therefore, the
particle size is also a factor that cannot
be ignored in theory. In this study, d50 is set to be 10um, 30um,
50um, 70um and 90um, respectively.
The thermal conductivity of the aluminum powder is
calculated.
(4) particulate material TCs
The particle material in this study mainly refers to the thermal
conductivity of the particle itself,
TCs. When TCs changes, ETCp will also change [20]. However, the
extent of the impact needs to be
analyzed. The present study performs the analysis by adjusting the
TCs condition in the software
calculation.
1.The influence of parameters
In this study, the control variable method is used to analyze the
parameters. Each time, only one
variable is changed to observe its influence on the thermal
conductivity. The powder used in the
calculation is spherical particles with random particle size
distribution and the medium is air at
atmospheric pressure. Figure 4 shows the calculation results.
Figure 4Trend of ETCp with parameters (a)(d) ETCp changes with
parameters. (e) ETCp
sensitivity analysis of parameter.
The calculation results of figure 4(a)(b)(c)(d) are all based on
spherical aluminum powder with
random particle size distribution and illustrate T, , d50 and TCS
has a reasonable trend consistency
with the thermal conductivity of the powder, which means that the
four parameters have an impact
on ETCP. However, the degree of impact is obviously different.
Therefore, it is necessary to
normalize the variables to study the influence degree of these four
parameters. It is assumed that the
sequences x1, x2, x3... xn are standardized as follows:
(7)
Where xi and x’ i denote the original variable and the unified
dimensionless variable, respectively.
Moreover, max{xi} and min{xi} are the maximum and minimum values of
variables when they
change, respectively. Figure 4(e) shows the results that after
treatment, the slopes of solid friction ε,
particle sizes d50 and temperature T are large and the following
conclusions can be drawn:
Firstly, the slop of TCs is approximately horizontal which means
the TCs has little effect on the
thermal conductivity of the powder, when the particle size is
randomly distributed. Therefore, in
practical application, when the requirements for heat conduction
accuracy are not high, and the
particle size distribution is random, the actual heat transfer
error caused by changing different
materials and the medium gas of powder can be ignored.
Second, the slope of solid friction is nearly vertical, which means
that the thermal conductivity
of the powder is highly sensitive to the compactness of the
deposit. Therefore, the solid fraction of
particles can be regarded as the core factor affecting the thermal
conductivity of particles.
2. Core factor confirmation
In order to verify the above mentioned viewpoint, two groups of
particle models of different
materials are established in the present study. One of group is
spherical aluminum powder (TCS =
240 W/mK) and the other one is 316L (TCS = 15W/mK) stainless steel.
Moreover, each group of
material particle models is divided into two kinds of particle
size, including 30um and 120um. Under
the same particle size and according to the different standard
deviation of the particle size
distribution, it also can be divided into equal particle size model
and nonequal particle size model.
Table 1 shows the basic information of powders. The model is
calculated at 27 . Figure 5 shows
the calculation results.
Table1: Basic information of Al and 316L powders
Materials Particle sizes d50(um) Solid fraction ε Equal particle
size yes or not
AL 30 0.5545 Yes
AL 30 0.5827 No
316L 30 0.5545 Yes
316L 30 0.5827 No
AL 120 0.5479 Yes
AL 120 0.5838 No
316L 120 0.5479 Yes
316L 120 0.5838 No
x x
£ £
£ ££ £

¢ = 
Figure 5. Comparison of ETCp results of equal particle size but
different particle size distribution powder. (a) model of unequal
size powder (b) model of equal size powder (c) Discoid display
of
contact surface of two kinds of stacking structures (d) Columnar
display of contact surface of two kinds of stacked structures (e)
The change of packing density of equal and unequal size packing
structure, and the trend of ETCp when TCs changes.(f) The relative
change of ETCp in astacking
structure and bstacking structure when the materials changes
respectively.
The following results are obtained from figure 5:
a. As the particle size increases, ETCP shows a rising trend, and
the rising range of particles with
equal particle size is significant.
b. Due to the influence of TCS, the thermal conductivity of Al
particles is higher than that of 316L
particles. However, according to the standard deviation of the
particle size distribution, the degree
of deviation is very different. The small and mediumsized figures
show that the powder with the
same particle size is significantly affected by the thermal
conductivity of the particle itself. However,
the influence of the powder with normal particle size distribution
is relatively small. It should be
indicated that the deviation shall not exceed 10%.
c. When the solid fraction of the packing model is compared with
the calculated heat conduction
coefficient, it is observed that trend of the two is not the same
and they even showing an opposite
trend. Compared with the nonequal size powder, the Solid fraction
of equal size powder is relatively
lower. However, its thermal conductivity is higher. This shows that
it is not accurate to regard the
solid fraction of particles as the core factor affecting the
thermal conductivity of particles.
d. The circular and cylindrical display of the particle contact
distribution of the stacking structure
with d50 of 30um is shown in Figures 6 (c)(d). It is observed that
the larger disk and the wider the
cylinder results in the larger the contact area between particles.
Therefore, it is found that under the
same d50, although the Solid fraction of the powder with equal
particle size is smaller, the contact
area between particles is larger. Meanwhile, from the Figures 6 (d)
it is obvious that as the contact
area between particles increases, the heat transfer channel between
particles becomes wider, the heat
transfer speed in particles is faster, and the calculated thermal
conductivity is larger. Therefore, it is
considered that the average contact area of particles is a more
important factor than the Solid fraction.
3. Empirical formula fitting of ETCp
In order to verify this statement, two groups of aluminum powder
with d50 in the range of
10um120um (equal particle size and nonequal particle size) are
selected to calculate the thermal
conductivity and the average contact area of particles. In the
present study, it is assumed that all
particles are spherical elastic rigid bodies, and the radius and
position information of each particle
(ri,xi,yi,zi) can be obtained in the process of establishing the
physical model.
Figure 6. Calculation diagram of particle contact area
As shown in Figure 6, it is assumed that in the case of contact
between two particles:
. The average particle contact area can be calculated by the
following equation:
(8)
Where s and dk denote the number of contact pairs of particles,
which are accumulated during the
calculation and the contact diameter, respectively.
(9)
(10)
Fig. 7 (a) shows that for powders with the equal particle size, the
average contact area and
densification have strong regularity with ETC, and the covariance
is 0.923 and 0.486, respectively.
For the powder with random particle size distribution, due to the
randomness of the particle size
distribution and stacking structure, the regularity of the average
contact area decreases. However,
the covariance is still 0.758. While, the compactness loses its
regularity. No matter from the data
display or covariance calculation, the correlation between Solid
fraction and ETCp is very random.
Therefore, it is concluded that the average contact area of
particles is more important than the
particle solid fraction.
The fitting function obtained by fitting the data points in figure
7 is described as follows:
ETC = 0.16 + 0.19(1exp(2.2aave)) (11)
In equation (11), when the temperature is room temperature,
aluminum powder is considered as the
standard powder, and the calculation formula of the thermal
conductivity is reduced to the average
k i jl r r< +
2
1
0.25
s
æ ö = ç ÷ è ø å
( )4 ( )( )( ) , ( ) 2k i j k k i j kd p p r p r p l l p r r l=  
 = + +
2 2 2( ) ( ) ( )k i j i j i jl x x y y z z=  +  + 
contact area of a variable particle (aave). Meanwhile, the
correlation between d50 of particles and the
average contact area is displayed in figure 7 (c).
Figure 7. (a)Calculation results of equal particle size powder
(b)Calculation results of nonequal particle size powder (c) the
correlation between d50 of particles and the average contact
area
It is observed that there is a strong correlation between d50 and
the average contact area of
particles, whether they are equal or randomly distributed.
Therefore, according to figure 8, the
correlation of randomly distributed powder between d50 and aave can
be obtained as follows:
(12)
Where, b0 = 0.02, b1 = 0.00192, b2 = 1.19e4 and d50∈(10um,
150um). Therefore, the correlation
between ETCP and d50 can be determined. Then, the experimental
values of other studies and the
present study are compared with each other when temperature is 27
degree[18, 2124]. Figure 8
shows the obtained results:
Figure 8. Comparison between theoretical data band and experimental
data. (a)Calculation high
limit (δ = 0.6), low limit (δ = 1.4) and base line. (b) Error
analysis of theoretical data band and
experimental data.
It is found that the experimental data is mostly nearby the base
line in figure 8(a). Actually, as shown
in Figure 8(b), the average relative error between the calculated
value and the experimental value is
2
0 1 50 2 50ave a b b d b d= + +
±20.9%, when d50 is 10150um, and the error is reduced to ±14.239%
when d50 is 20100um.
However, the error of smaller particle size and larger particle
size is relatively large even up to 55%.
Therefore, in order to further improve the accuracy, considering
the error of the experimental results
and the influence of the thermal conductivity of the particles
themselves, the adjustment coefficient
δ (0.6 ≤ δ ≤ 1.4) is introduced as equation 13 and δ = 1 when the
particle material is aluminum (TCS
= 240 W/mK). Common materials and corresponding δ value are shown
in the table 2.
Table2: Common metal materials and corresponding δ value
Materials Ti6Al4V 316Lsteel Fe W Al Cu Ag
δ 0.6 0.680 0.749 0.925 1 1.349 1.4
Furthermore, according to Samuel et al and the experimental results
obtained in this study [20],
the correlation between ETCp and temperature is approximately
linear as follows:
ETCp=ETC0+λT (14)
Where ETC0 can be obtained from equations 12 and 13, T is the
temperature in , λ = 2.78112e4
and the relative error is ±30%. Therefore, according to equations
12,13 and14, a ETC space (random
particle sizes distribution, standard atmospheric pressure, without
concern gas medium changing) is
shown in the figure 9 which contains the thermal conductivity of
any metal sphere powder at any
temperature when d50 is 10150um and the relative error in high
temperature is ±50%.
Figure 9. ETC space contains the thermal conductivity of any metal
powder at any temperature when d50 is 10150um.
Conclusion
In the present study, based on the spherical aluminum powder, the
relationship between the
parameters and the thermal conductivity of the powder is studied.
The main findings were
summarized as follows:
1. The slop of TCs with ETCp is approximately horizontal which
means the TCs has little effect on
the thermal conductivity of the powder, when the particle size is
randomly distributed. Therefore,
(13) 2
0 0 1 50 2 50(0.16+0.19(1 exp( 2.2( )))ETC b b d b dd=   +
+
in practical application, when there no strict requirements for
heat conduction accuracy, and the
particle size distribution is random, the actual heat transfer
error caused by changing different
materials the medium gas of powder can be ignored.
2. Temperature T, solid fraction and particle sizes d50 all of them
have a great influence on thermal
conductivity of powder (ETCp). However, these parameters have
different effects on ETCp which is
very sensitive to the change of solid fraction .
3. By calculated the ETCp with the same average particle size but
different particle size distribution,
it is found that solid fraction as a core parameter is not
accurate. Actually, the average contact area
between particles(aave) is the key factor that affects the
efficiency of heat conduction of powder
which means the change trend of ETCp can be relatively accurate
described by aave.
4. Through calculation, it is found that aave and average particle
d50 size also have a close nonlinear
relationship.
Based on the above four points, a simple and efficient calculation
model of the ETCp is
established. The simplicity of this model originates from its low
input parameters. In fact, only
parameter d50 is required for the established model. This parameter
can be found in the document
as the standard parameter of a commercial powder. Meanwhile,
concern the effect of temperature
and TCS, a ETCp space (random particle sizes distribution, standard
atmospheric pressure, without
concern gas medium changing) is established which contains nearly
all metal sphere powder (d50
10um150um) ETCp in 25 to 1000, and the error is no more than 20.9%
in the room temperature
and 50% in high temperature.
Acknowledgements
Not applicable.
Authors’ Contributions
YZ and HZ were in charge of the whole trial; YZ wrote the
manuscript; SJ and JC assisted with
sampling and data analyses. All authors read and approved the final
manuscript.
Authors’ Information
Yizhen Zhao, born in 1993, is currently a doctoral candidate at
School of Mechanical Engineering,
Xian Jiaotong University, China.
Hang Zhang, born in 1985, is currently an associate professor at
School of Mechanical Engineering,
Xian Jiaotong University, China. He received his doctor degree from
QingHua University, China,
in 2014. His research interests include additive manufacturing and
high entropy alloy.
Jianglong Cai, born in 1996, is currently a master candidate School
of Mechanical Engineering,
Xian Jiaotong University, China.
Shaokun Ji, born in 1996, is currently a master candidate School of
Mechanical Engineering, Xian
Jiaotong University, China.
Dichen Li, born in 1964, is currently a professor at School of
Mechanical Engineering, Xian
Jiaotong University, China.
Funding
This work was financially supported by the National Natural Science
Foundation of China (No.
51975459) and Shaanxi Natural Science Foundation
(No.2017JM5046).
Competing Interests
Author Details
1 School of Mechanical Engineering, Xi’an Jiaotong University,
Xi’an 710049, China. 2 School of
Mechanical Engineering, Xi’an Jiaotong University, Xi’an 710049,
China. 3 School of Mechanical
Engineering, Xi’an Jiaotong University, Xi’an 710049, China. 4
School of Mechanical Engineering,
Xi’an Jiaotong University, Xi’an 710049, China. 5 State Key
Laboratory of Manufacturing Systems
Engineering, School of Mechanical Engineering, Xi’an Jiaotong
University, Xi’an 710049, China
References
[1] Wu, H., N. Gui, Numerical simulation of heat transfer in packed
pebble beds: CFDDEM
coupled with particle thermal radiation. Int. J. Heat. Mass.
Transf. 110 (2017) 393405.
[2] Norouzi, H.R., R. Zarghami, and N. Mostoufi, New hybrid CPUGPU
solver for CFDDE
M simulation of fluidized beds. Powder. Technol. 316 (2017)
233244.
[3] Gan, J., Z. Zhou, and A. Yu, Effect of particle shape and size
on effective thermal conducti
vity of packed beds. Powder. Technol. 311(2017) 157166.
[4] Matsushita, M., M. Monde, and Y. Mitsutake, Predictive
calculation of the effective therm
al conductivity in a metal hydride packed bed. Int J Hydrogen
Energy. 39 (2014) 971897
25.
[5] You, E., X. Sun, An improved prediction model for the effective
thermal conductivity of c
ompact pebble bed reactors. Nucl. Eng. Des. 323 (2017)
95102.
[6] Cundall, P.A. and O.D.L. Strack, Discrete NumericalModel for
Granular Assemblies. Geo
technique 29 (1979) 4765.
[7] Bahrami, M., M.M. Yovanovich, and J.R. Culham, Effective
thermal conductivity of roug
h spherical packed beds, Int. J. Heat. Mass. Transf. 49 (2006)
36913701.
[8] Boudenne, A., L. Ibos, Thermophysical properties of
polypropylene/aluminum composites
. J. Polym. Sci., Part B: Polym. Phys. 42 (2004). 722732.
[9] Bahrami M , Yovanovich M M , Culham J R . A Compact Model for
Spherical Rough Con
tacts[C]// Asme/stle International Joint Tribology Conference.
ASME. J. Tribol. 127 (2005
) 884889.
[10] Holotescu, S. and F.D. Stoian, Prediction of particle size
distribution effects on thermal c
onductivity of particulate composites. Materialwiss. Werkstofftech.
42 (2011) 379385.
[11] Moayeri, M. and A. Kaflou, Effect of powder shape on effective
thermal conductivity of
Cu–Ni porous coatings. J. Mater. Res. Technol. 7 (2018)
403409.
[12] Zhang, H., Y. Zhao, A 3D discrete elementfinite difference
coupling model for predictin
g the effective thermal conductivity of metal powder beds. Int. J.
Heat. Mass. Transf. 132
(2019) 110.
[13] ZainulAbdein, M., S. Azeem, Computational investigation of
factors affecting thermal
conductivity in a particulate filled composite using finite element
method. Int J Eng Sci 5
6(2012) 8698.
[14] H. Zhang, W.Z.F, Experimental study of the thermal
conductivity of polyurethane foams
, Appl. Therm. Eng. 115 (2017) 528–538.
[15] H. Zhang, Y.L., W. Tao, Effect of radiative heat transfer on
determining thermal conducti
vity of semitransparent materials using transient plane source
method, Appl. Therm. Eng.
114 (2017) 337–345.
[16] G.P. Joshi, N.S.S., R. Mangal, Temperature dependence of
effective thermal conductivity
and effective thermal diffusivity of NiZn ferrites, Acta
materialia 51 (2003) 2569–2576.
[17] Zhang, H.W., Q. Zhou, A DEM study on the effective thermal
conductivity of granular as
semblies, Powder. Technol. 205(2011) 172183.
[18] Kohout, M., A.P. Collier, and F. Štpánek, Effective thermal
conductivity of wet particle
assemblies, Int. J. Heat. Mass. Transf. 25 47(2004)
55655574.
[19] Xu, W.X., Z. Lv, Effects of particle size distribution, shape
and volume fraction of aggre
gates on the wall effect of concrete via random sequential packing
of polydispersed ellips
oidal particles, Phys. A 392 (2013) 416426.
[20] 1.Sih, S. S. & Barlow, J. W. Measurement and prediction of
the thermal conductivity of p
owders at high temperatures. Solid Freeform 400 Fabrication
Symposium Proceedings 32
1–329 (1992).
tallic powders, J Appl Phys 97(2005) 024905.
[22] Wei, L.C., L.E. Ehrlich, Thermal conductivity of metal powders
for powder bed additive
manufacturing, Addit. Manuf. 21(2018) 201208.
[23] Chua, B., Lee, H. Ahn, D. Estimation of Effective Thermal
Conductivity of Ti6Al4V P
owders for a Powder Bed Fusion Process Using Finite Element
Analysis, Int. J. Precis. En
g. Manuf. 19 (2018) 257–264.
[24] K Bala, P R Pradhan, Effective thermal conductivity of copper
powders, J. Phys. D: Appl
. Phys. 22(1989) 1068.
Figure 2
Figure 3
The heat transfer forms in particle model and the thermal
resistance composition in particle contact area.
Figure 4
Trend of ETCp with parameters (a)(d) ETCp changes with parameters.
(e) ETCp sensitivity analysis of parameter.
Figure 5
Comparison of ETCp results of equal particle size but different
particle size distribution powder. (a) model of unequal size powder
(b) model of equal size powder (c) Discoid display of contact
surface of two kinds of stacking structures (d) Columnar display of
contact surface of two kinds of stacked structures (e) The change
of packing density of equal and unequal size packing structure, and
the trend of ETCp when TCs changes.(f) The relative change of ETCp
in astacking structure and bstacking structure when the materials
changes respectively.
Figure 6
Figure 7
(a)Calculation results of equal particle size powder (b)Calculation
results of nonequal particle size powder (c) the correlation
between d50 of particles and the average contact area
Figure 8
Comparison between theoretical data band and experimental data.
(a)Calculation high limit (δ = 0.6), low limit (δ = 1.4) and base
line. (b) Error analysis of theoretical data band and experimental
data.
Figure 9